IOSR Journal of Applied Chemistry (IOSR-JAC)
e-ISSN: 2278-5736.Volume 4, Issue 4 (May. – Jun. 2013), PP 42-46
www.iosrjournals.org 42 | Page
XRF Studies for Chemical Composition and Molecular Formula
of Jharkhand Bentonite
, Vats Amitabh 2
, Babita Kumari3
, Bivekanand mishra4
(Department of Chemistry, Bhagwant University, Ajmer, Rajasthan, India)
(D.N.S College, Rajoun, Banka, India)
(Mahila College, Godda, Jharkhand, India)
(Dept. of Chemistry, T.M. Bhagalpur University, Bhagalpur, Bihar, India)
Abstract : The present work is an endeavor to study and trace out good quality bentonite having commercial
values from the different parts of Jharkhand hills particularly Sahibganj, Dumka, Godda, Deoghar, Lohardagga
and Daltaganj. The work involved survey and sample collection of bentonite samples from the region and their
analysis using X-Ray Fluorescence (XRF). The XRF analysis of twenty three samples was done to obtain
chemical composition, which was then used for derivation of the theoretical molecular formula. XRF technique
has been used for the first time for determining the Chemical Composition of bentonite of Jharkhand hills. The
analysis indicates that all the samples except one are good quality bentonites.
Keywords - Bentonite, Chemical Composition, Jharkhand Bentonite, Theoretical formula
India is facing the problem of fluoride in ground water and now even in Ganga water. Provisioning of
drinking water to vast population of not only this country, but world as a whole, has put a challenge to the
chemists. Recent observation of Arushi Gupta [1, 2] shows that bentonite of Rajmahal hill may be a suitable
alternative for methods of removal of fluoride from water, particularly, potash alum used in the well-established
Nalgonda method. It has been observed that the drinking water supplied to the people of Bhagalpur after
treatment of Ganga water contains poisonous metal Aluminium causing Cancer and Alzheimer.
Scanty literature [3-9] is available regarding the quantity of vast deposits of Bentonite in hills of
Jharkhand. In continuity of the research information available on the Bentonite from Rajmhal hill and their good
quality and commercial values, the work has been extended for the survey and sample collection from the
different parts of Jharkhand hills particularly to Sahibganj, Dumka, Godda, Deoghar, Lohardagga and Daltaganj
for their studies to trace out good quality bentonite having commercial values and their properties for fluoride
removal and to use them as an alternative for potash alum in Nalgonda method.
Twenty three samples were collected after thorough survey in the woods of hills of Jharkhand under
the team leader Dr. Shashi Shekhar Singh (Geology Department, M.S. College, Bhagalpur) along with team
members Dr. Vats Amitabh (Rajoun, Banka) and Dr. Babita Kumari (Mahila College, Godda). The samples
were prepared and packed as per the methods reported in literature earlier . X-Ray Fluorescence (XRF)
analysis of these samples was done with the help of Philips PW1480 XRF Spectrometer at Sophisticated
Analytical Instrument Facility (SAIF), Gauhati University, Guwahati. Chemical Analysis of the Bentonite
samples was undertaken by employing the computerized sequential X-Ray Fluorescence Spectrometer. The
Philips X-Ray Spectrometer has Rh, Cr-Au X-Ray tube and can identify elements from Fluorine to Uranium. It
has two detectors namely Flow Proportional Counter & Scintillation Counter. For the purpose of analysis of
Clay minerals it uses silicate rock, cement, limestone as standard reference material. The chemical composition
of the samples under test was analyzed using silicate rock as standard reference material. The composition data
obtained were verified by the data obtained by standard methods of literature [11-15]. The chemical
composition has been used for derivation of theoretical molecular formula of these samples. The samples were
marked AB (Arushi Bentonite) in place of SRHB (Santhal Pargana Rajmahal Bentonite) to distinguish between
regions of collection of samples. They are recorded in Table-1. The chemical composition data obtained by XRF
is presented in Table-2. The percentage composition of the Bentonite of this region is tabulated in Table-3. The
method of calculation of theoretical formula has been given in Table-4. Theoretical formula of Bentonite of this
region has been recorded in Table-5.
III. RESULT AND DISCUSSION
On analysis the percentage composition data of Table-3, it has been found that high percentage of
Silica, even more than sixty percent is present in AB7 (Jashidih), AB2, AB11 (Sahibganj) and AB17 (Dumka)
XRF Studies for Chemical Composition and Molecular Formula of Jharkhand Bentonite
www.iosrjournals.org 43 | Page
and this data is comparatively higher than the data reported for Rajmahal hills Bentonite1
and the literature
values present in Table-2. Other bentonite samples have lower limit of 50.93 percent and higher limit of 59.87
percent which is comparable with the data for Silica in Rajmahal Bentonite and the literature values for
Bentonite of U.S.A, Canada, and some other state of India.
The Silicon Dioxide and Alumina ratio ranges from 1.69 for AB23 to 3.67 for AB7 in comparison with
the ratio for Rajmahal Bentonite having this value from 1.07 to 2.0 approximately. Again AB11 has this ratio
equal to 6.76 which is abnormally high. For Yellow Stone of U.S.A., this ratio is 3.03 and for California it is
4.60 where as for Barmer sample it is 2.90 but for Bhimbar sample it is 3.0.
Another important constituent of Montmorillonite is Alumina. The percentage composition of Alumina
ranges from 17.92 (AB7) to 31.84 (AB23) with exceptional values like 11.34 (AB11) and 14.49 (AB15). Other
values of all Bentonite samples of this range AB1, AB2, AB4, AB5, AB6, AB8, AB9, AB11, AB12, AB13,
AB14, AB16, AB17, AB18, AB19, AB20, AB21, AB22 and AB23 are well comparable with the values for
Rajmahal hill Bentonite having Alumina percentage varied from 18.98 to 33.06. These values are also,
comparable with the literature values present in Table-2. California sample contains only 12.76 percent of
Alumina as compared to AB11 of Sahibganj having 11.34 percent and AB15 of Godda having 14.49 percent.
The higher percent of Silica and lower percent of Alumina in AB11 gives an indication of this sample
having less amount of Montmorillonite and may be declared as poor quality Bentonite. The Silicon Dioxide and
Alumina Ratio for Bentonite of this range varies from 1.69 to 3.67 for 20 samples of this zone. The abnormal
highest value of 6.76 for AB11 confirms our earlier conclusion regarding this sample. Other values reported in
the literature are well comparable with the present values/ the values for Bentonite of the world.
The ratio for Aluminium to Ferric Oxide ranges from 2.78 to 7.12 for 18 samples whereas the highest
value of 17.30 for AB 13 and 16.92 for AB11 are seen. The percentage data for MnO, MgO, CaO, Na2O and
K2O are well comparable with literature values of Bentonite of various states of India and other countries. The
higher percentage of Titanium Dioxide is 3.41 and 3.81 percent in the sample AB18 and AB19, more than one
percent of Titanium Dioxide is present in almost all samples of this region, AB11 is again having only the
lowest value of 0.15 percent.
Theoretical and Molecular Formula Of Bentonite Of Jharkhand: Standard and established
method of calculation of theoretical formula of literatue [1, 17, 18] was used for these Bentonites. Method of
calculation of theoretical molecular formula of one sample has been recorded in Table-4. Using this method the
theoretical molecular formula of other samples have been calculated and represented in Table-5.
The general theoretical structural formula of half unit cell structure of Bentonite may be written as
(SiaAlb)(AlcFedMge)CafNagKhO10(OH)2. The value for a, b, c, d, e, f, g, h are tabulated in Table-5. While
calculating the theoretical molecular formula of Bentonite, the percentage of Titanium Dioxide was not taken
into consideration as, the main constituent of Bentonite is Montmorillonite, and Titanium Dioxide is not the
constituent part of Montmorillonite [10, 14]. The formula of Rajmahal bentonite has been reported in literature1
and compared with the formula reported here. The structural formula of Rajmahal bentonite is
CafNagKhO10(OH)2 where a=2.57 to 3.57, b= 0.42 to 1.43, c=1.14 to 1.67, d = 0.10 to
0.56, e= 0.01 to 0.53, f=0.03 to 0.46, g=0.12 to 1.23 and h= 0.03 to 0.53.
The values of a, b, c, d, e, f, g, h for Jharkhand samples are in the range; a = 3.49 to 4.77, b = 0.07 to
0.9, c = 0.5 to 1.88, d = 0.03 to 0.41, e = 0.005 to 0.37, f = 0.0007 to 0.23, g = 0.14 to 0.34 and h = 0.01 to 0.19.
The maximum value of 'a' for Jharkhand bentonite is 4.51 which is more than the maximum value of a=3.57 for
Rajmahal bentonite. However, only five samples AB1, AB2, AB7, AB11 and AB15 have the 'a' value above 4.
Balance 18 samples have these values comparable to Rajmahal Bentonite. The combined value of ‘b’ and ‘c’ for
reported sample is 2.39 which is nearly equal to combined value of ‘b’ and ‘c’ = 3.1 for Rajmahal bentonite. The
value of e, f and h in the present samples, are lesser than the values reported for the Rajmahal bentonite.
Twenty three samples of bentonite were collected from the different parts of Jharkhand hills after
thorough survey, particularly for examining their properties to trace out good quality bentonite having potential
of fluoride removal from water, thereby offering a low cost method for provisioning potable water to rural
population of Jharkhand region. The XRF analysis was undertaken on the samples to determine their chemical
composition and their theoretical molecular formula. The results were compared with the literature values and it
has been ascertained that all the samples except one are good quality bentonite. The chemical composition of
bentonites of Jharkhand hills is also comparable to that of Rajmahal hills and can be used for defluoridation of
XRF Studies for Chemical Composition and Molecular Formula of Jharkhand Bentonite
www.iosrjournals.org 44 | Page
The author expresses gratitude to SAIF Guwahati, Gauhati University for undertaking the requisite analysis
in their testing facility and Lt Cdr Ankush Gupta for generous financial assistance.
 Arushi Gupta, M. Kumar, A.K. Jha, B.K. Mishra, J. Choudhary and Bivekanand Mishra, Chemical Composition and Molecular
Formula of Rajmahal Bentonite (Jharkhand) Asian Journal of Chemistry, 23(12), 2011, 5491-5494.
 Arushi Gupta, M. Kumar, J. Choudhary and Bivekanand Mishra, TGA and TG studies of Rajmahal Hills Bentonites of Jharkhand in
India, Communicated to Journal of Indian Chemical Society, 2013.
 H.N. Siddique and D.P. Bahl, Geology of the Bentonite Deposits of Barmer District, Rajasthan, Memoirs of the Geological Survey
of India, 96, 1965.
 Satyabrat, K Balu and K. T. Thomas, Transformation of naturally occurring interstratified Radioactive Waste, BARC, 1971.
 C.S. Raja Rao, Geological Survey of India progress report on Santhal Parganas, Bihar, for the season 1954, Rec Geol. Surv. Ind.,86,
 B. Chaliha, Utilizationof Indian bentonite in the refining of vegetable oils, Sci. Cult., 21, 1955,161.
 S.K. Guha and Sudhir Sen, A study of the physico-chemical properties of Bihar bentonites, Trans. Ind. Ceram. Soc., 20, 1961,73-
 B.M. Bishnui and R. Prasad, Mineralogical nature of some Indian clays. Part II- Clays from Lamehtaghat, Khandagiri, Tinapahar
and Hathi-ki-Dhani, Bull. Cent. Glass Ceram. Res Inst., 7, 1960, 11-28.
 K.L. Bhola, Bentonite in India, Quart Jour. Geo. Min Met Soc. Ind., 19, 1947, 55-77.
 J. Choudhary, PhD thesis, T.M Bhag. Univ., 1985.
 S. Ambi, M. Tech. Dissertation, IIT Delhi, 1977.
 S. Ambi, N.K. Jha, M.M. Prasad, and Bivekanand Mishra, Study on Montmorillonite from Santhal Pargana district in Bihar, J. Ind.
Chem. Soc., 55, 1978, 1077-1079.
 N.K. Jha, Bivekanand Mishra, M.M. Prasad, Ind. Courier, 8, 1976, 1.
 B.K. Mishra, PhD thesis, T.M. Bhag. Univ., 2001.
 S.S. Mishra, PhD thesis, S.K.M. Univ., 2008.
 A.K. Jha, PhD thesis, S.K.M. Univ., 2011.
 S. Calliere and S. Henin, Mineralogic Des. Agrles (Masson & Co., 1963).
 N.K. Jha, Private Communication, August 1982, Chem. Dept., IIT Delhi.
Table 1 Locations From Where Samples Were Collected
S. No. Sample No. Location
1. AB 1 Bakudih
2. AB 2 Sahibganj
3. AB 3 Bakudih
4. AB 4 Bakudih
5. AB 5 Deoghar
6. AB 6 Chitra
7. AB 7 Jasidih
8. AB 8 Dumka
9. AB 9 Goddha
10. AB 10 Sahibganj
11. AB 11 Sahibganj
12. AB 12 Godda
13. AB 13 Daltaganj
14. AB 14 Daltaganj
15. AB 15 Goddha
16. AB 16 Goddha
17. AB 17 Dumka
18. AB 18 Dumka
19. AB 19 Dumka
20. AB 20 Goddha
21. AB 21 Daltaganj
22. AB 22 Lohardaga
23. AB 23 Dumka
TABLE 2 PERCENTAGE COMPOSITION OF BENTONITE FROM LITERATURE
S No. Sample SiO2 Al2O3 Fe2O3 TiO2 CaO MgO K2O Na2O
1. Harwecha 47.82 15.88 9.8 1.34 2.4 2.23 0.8 2.29
2. Hati Singh Ki dhani 50.86 20.99 7.2 1.32 Tr 3.04 0.56 1.13
3. AkliGiral 47.25 18.27 9.54 1.24 1.07 1.41 0.96 1.75
4. AkliThumbliGiral 57.35 16.98 7.34 1.28 1.54 1.54 1.55 1.2
5. ThumbliAkli 49.99 20.11 6.79 1.34 0.68 1.23 0.82 3.24
6. Bisala 46.38 25.15 8.4 1.7 Tr Tr 0.56 1.46
7. Bhadres 45.77 19.06 12.6 2.19 Tr 3.11 0.81 1.23
8. Mahwar 41.12 19.58 12.6 1.74 1.16 2.46 0.8 1.16
9. USA 59.92 19.78 2.96 2.96 0.64 1.33 0.57 2.06
10. Canada 53.96 15.44 1.31 1.31 0.8 6.99 0.54 -
11. Akli 54.9 19.4 6.8 6.8 0.2 - 0.9 2.1
12. Jammu and Kashmir 52.4 17 1.8 1.8 1.9 1.3 - 2.51